| ||Format||Pages||Price|| |
|4||$41.00||  ADD TO CART|
|Hardcopy (shipping and handling)||4||$41.00||  ADD TO CART|
Significance and Use
This test method is an accelerated test to determine if a copper alloy product will be susceptible to stress-corrosion cracking when exposed to a particular atmospheric condition during service with the appropriate risk level
This test method is generally intended to determine if a copper alloy product will crack because of internal stresses when subjected to the test, and is not intended for testing assemblies under applied stress. If used for this purpose, it shall be for information only and not a cause for rejection of the assembly, its component parts, or the original mill product.
1.1 This test method describes a procedure to determine the presence of residual stresses in wrought copper alloy products that may lead to stress corrosion cracking. An ammonia vapor atmosphere is used as an accelerated test.
1.2 This test method is only suitable for products fabricated from copper alloys that are known to be susceptible to stress corrosion cracking in ammonia vapor atmospheres. It is intended to create an environmental condition of reproducible severity.
Note 1—It is well known that the critical step in the cracking mechanism is the development of an environment in the condensate film that occurs on the surface of the test specimen, and is rich in copper complex ions.
1.3 The severity of this test method depends upon the pH of the corrosive solution. In Annex A1 are given four different atmospheres to which the product may be exposed, and the appropriate pH of the solution to be used for the test, depending on the risk level associated with the intended application.
1.3.1 The appropriate pH value for the test shall be specified in the product specification, or as per established agreement between the supplier and purchaser, with respect to the alloy and its intended application.
1.4 Units—The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
B154 Test Method for Mercurous Nitrate Test for Copper Alloys
B846 Terminology for Copper and Copper Alloys
D1193 Specification for Reagent Water
ICS Number Code 77.120.30 (Copper and copper alloys)
UNSPSC Code 41114604(Corrosion testers)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM B858-06(2012), Standard Test Method for Ammonia Vapor Test for Determining Susceptibility to Stress Corrosion Cracking in Copper Alloys, ASTM International, West Conshohocken, PA, 2012, www.astm.orgBack to Top